Feb 27, 2004 - 1Department of Materials Science and Engineering, Virginia Tech, ... Laboratory, 1800 E. Paul Dirac Drive, Tallahassee, Florida 32310, USA.
PHYSICAL REVIEW B 69, 064114 共2004兲
Magnetic-field-induced phase transition in BiFeO3 observed by high-field electron spin resonance: Cycloidal to homogeneous spin order Benjamin Ruette,1 S. Zvyagin,2 A. P. Pyatakov,3 A. Bush,4 J. F. Li,1 V. I. Belotelov,3 A. K. Zvezdin,3 and D. Viehland1 1
Department of Materials Science and Engineering, Virginia Tech, Blacksburg, Virginia 24061, USA The National High Magnetic Field Laboratory, 1800 E. Paul Dirac Drive, Tallahassee, Florida 32310, USA 3 Institute of General Physics, Russian Academy of Science, Vavilova St., 38, Moscow 119991, Russia 4 Moscow State Institute of Radio Engineering, Electronics and Automation (Technical University), Vernadskii Prospect, 78, Moscow 117454, Russia 共Received 24 April 2003; revised manuscript received 29 September 2003; published 27 February 2004兲 2
Bismuth ferrite is a magnetoelectric material, which simultaneously has polarization and spin orders. We have used electron spin resonance 共ESR兲 as a local probe of the magnetic order in the magnetic-field range of 0–25 T, in the frequency domain of 115–360 GHz, and at a temperature of 4.2 K. The data reveal significant changes in the ESR spectra with increasing field, which have been analyzed by taking into account the magnetic anisotropy of the crystal and a magnetoelectric Dzyaloshinsky-Moria-like interaction. The results demonstrate an induced phase transition from an incommensurately cycloidal modulated state to one with homogeneous spin order. DOI: 10.1103/PhysRevB.69.064114
PACS number共s兲: 77.80.⫺e, 75.25.⫹z, 75.80.⫹q
Multiferroic materials have two order parameters. They can be spontaneous polarization 共ferroelectric or antiferroelectric兲 and a spontaneous magnetization 共ferromagnetic or antiferromagnetic兲.1 The magnetoelectric effect is the coupling between the spontaneous polarization P s and the spontaneous magnetization M s . Phenomenologically, this coupling can be either mediated by linear, biquadratic, or even higher-order exchanges.2 One of the first multiferroic materials found was BiFeO3 , 3 which has a perovskitelike structure. It has been demonstrated that BiFeO3 has two order parameters:1 共i兲 a polarization 共ferroelectric兲 ordering with a high Curie temperature T C of 1103 K;3,4 and 共ii兲 a spin 共antiferromagnetic兲 ordering of the G type with a magnetic transition temperature T N of 643 K.5–7 Clearly, the spin and polarization orderings are driven by different modes, as the phase-transition temperatures are significantly different. The average crystal lattice of BiFeO3 is a rhombohedrally distorted perovskite structure,5,7–12 which belongs to the space group R3c 共or C 3V 6 ), as shown in Fig. 1共a兲. The hexagonal unit-cell parameters are a⫽5.58 Å and c⫽13.9 Å. In this structure, along the threefold pseudocubic 关 111兴 c rotation axis, the Bi3⫹ and Fe3⫹ cations are displaced from their centrosymmetric positions. This centrosymmetric distortion is polar, and results in a spontaneous polarization ( P s ), as illustrated in Fig. 1共a兲. Previous investigations of the polarization behavior of oriented single crystals have shown a P s of 0.035 C/m2 along the 关 001兴 c at 77 K.10 However, recent investigations of single crystalline thin layers fabricated by pulsed laser deposition have shown a much higher P s along the 关 001兴 c and 关 111兴 c , approaching values of 0.6 C/m2 共Ref. 13兲 and 1 C/m2 共Ref. 14兲 at room temperature, respectively. Antiferromagnetic (T N ⬃643 K) BiFeO3 has weak magnetism at room temperature.1 The spin is provided by the transition-metal cation Fe3⫹ . Spins in the neighboring atoms 0163-1829/2004/69共6兲/064114共7兲/$22.50
are antiparallel, leading to an antiferromagnetic ordering of the G type.1,7 In this arrangement, the Fe3⫹ cations are surrounded by six nearest Fe3⫹ neighbors, with opposite spin directions. Figure 1共b兲 shows the hexagonal representation of the spin structure of BiFeO3 . In this structure, the hexagonal 关 001兴 h direction is equivalent to the pseudocubic 关 111兴 c , about which axis there is a threefold rotation; and about the hexagonal 关 110兴 h , there is a mirror plane. Thus along the 关 001兴 h / 关 111兴 c , BiFeO3 has antiferromagnetic order, as illustrated in Fig. 1共b兲. Microscopically, the antiferromagnetic spin order is not homogenous for BiFeO3 single crystals. Precise neutrondiffraction studies15,16 have revealed an incommensurately modulated spin structure which manifests itself as a cycloid with a long wavelength of ⬃600 Å. In the incommensurate phase, the periodicity of the spin polarization is incommensurate with the crystallographic lattice parameters. The cycloidal spin structure has been shown to be directed along 关 110兴 h . The existence of the incommensurate cycloid has also been confirmed by line-shape analysis of nuclear magnetic resonance 共NMR兲 spectra.17,18 In BiFeO3 , the spin profile is nearly sinusoidal and the phase of the modulation is a linear function of the space coordinate in the direction of the modulation.15,19 However, temperature-dependent NMR studies have revealed that the spin profile becomes increasingly anharmonic as the temperature is decreased.17 Similar phenomena are observed in dielectrics where spatial profiles of polarization can be strongly anharmonic near the temperature of phase transition to a commensurate polar state, which consists of nearly commensurate regions separated by domain walls 共i.e., solitons兲 where the phase of the order parameter changes abruptly. In addition, the spin profile of BiFeO3 becomes anharmonic with increasing magnetic field H. At higher fields of H⬎18 T, an induced phased transition has been reported.20–22 Previously, in other materials, changes in the spatial profile of incommensurate structures,23–25 in soliton density,23,26,27 and soliton dimensionality (1⫺q vs 3⫺q) 共Refs. 28 and 29兲 with increasing magnetic and/or electric field have been reported.
©2004 The American Physical Society
PHYSICAL REVIEW B 69, 064114 共2004兲
BENJAMIN RUETTE et al.
due to the fact that the average value of the projection of the antiferromagnetic vector in the cycloidal structure is zero. However, the cycloidal structure does not prevent manifestation of the quadratic magnetoelectric effect.38 The spin cycloidal structure that prevents the linear magnetoelectric effect from being observed can be destroyed by high magnetic field. Application of high magnetic field can induce a phase transition from a spatially modulated spin structure to one with a homogeneous spin order. Previously, an induced phase transition and the appearance of a linear magnetoelectric effect have been reported by polarization measurements under a pulse magnetic field of 20 T.20–22 Electron spin resonance 共ESR兲 has been shown to be a very powerful tool for the study of magnetic excitation and phase transitions in solids.39,40 The main purpose of this investigation was to study the magnetic excitation spectrum of BiFeO3 crystals over a broad frequency range under steady magnetic fields up to 25 T. It was anticipated that this investigation would provide a more thorough and reliable understanding of magnetic-field-induced phase transitions and magnetoelectric coupling at high magnetic fields in BiFeO3 . II. EXPERIMENTAL PROCEDURE
FIG. 1. 共a兲 Crystal lattice of BiFeO3 , illustrating rhombohedral units and hexagonal cell. The direction of spontaneous polarization is illustrated in this figure. 共b兲 Hexagonal representation of spin structure of BiFeO3 . Both the antiferromagnetic order and spin rotation planes are shown in this figure.
The intrinsic spin-phonon coupling is generally small,1 as it involves a relativistic interaction between the two order parameters P s and M s . Phenomenologically, the linear exchange between the two in the Landau-Ginzburg equation of state, i.e., P i ⫽Q i j M j , inherently involves a coupling between the linear power of a polar tensor and a linear power of an axial tensor.30–37 This intrinsic linear coupling coefficient Q i j does not have a normal symmetric tensor matrix as a solution. Rather, the linear magnetoelectric exchange must have an antisymmetric component in its property tensor,30–37 in addition to the usual symmetric one. In BiFeO3 , the conventional Dzyaloshinksy-Moria interaction is zero. It is forbidden by the space-group symmetry. A linear magnetoelectric Dzyaloshinksy-Moria-like interaction is allowed by the 3m magnetic point group.34 Nevertheless, polarization measurements have shown that it is not observed in BiFeO3 when the cycloidal spin structure is present.20–22 The magnetoelectric effect is averaged to zero
Bismuth ferrite single crystals were grown by a flux method from a Bi2 O3 -Fe2 O3 -NaCl melt. Single crystals were oriented along the 关 001兴 c . Specimens were cut into dimensions of 1⫻1⫻0.5 mm3 . The structure was rhombohedral 共or hexagonal兲 and the crystal lattice parameters were a⫽b⫽c⫽5.61 Å and ␣ ⫽89.28° 共or a⫽5.58 Å and c ⫽13.9 Å). ESR is an extremely powerful tool to test magnetic excitation spectra in solids, providing important information on a magnetic structure and main parameters of the effective spin Hamiltonian. In order to test the field-induced phase transition in BiFeO3 , high-field ESR measurements were performed using the submillimeter facility at the National High Magnetic Field Laboratory 共NHMFL, Tallahassee, FL兲, in fields up to 25 T. Investigations have been done in the frequency range of 115–360 GHz. Quasicontinuously retuned sources of millimeter and submillimeter wave radiation, backward wave oscillators, were used. Transmission-type ESR spectrometer with oversized cylindrical waveguides and a sample holder in the Faraday configuration 共with a wave propagation vector parallel to the external field兲 was employed. A high-homogeneity 共12 ppm/cm DSV兲 magnetic field was produced by the 25-T hysteresis-free resistive Bitter-type W. M. Keck magnet. In our experiment, the magnetic field was oriented along the pseudocubic 关 001兴 c direction. Since absorption lines were relatively broad, an optical modulation of the microwave power was used. The spectra were recorded during the magnetic field sweeping. A low noise, wide frequency range, InSb hot electron bolometer, operated at liquid-He temperatures served as a detector. Experiments were performed at a temperature of 4.2 K. III. ESR SPECTRA
Figure 2 shows the ESR signal as a function of magnetic field for 0⬍H⬍25 T, taken at various frequencies between
PHYSICAL REVIEW B 69, 064114 共2004兲
MAGNETIC-FIELD-INDUCED PHASE TRANSITION IN . . .
FIG. 3. Electron spin resonance frequency as a function of magnetic field H (T⫽4.2 K).
The maximum of the absorption has been chosen to indicate the resonance field. Clearly, there is more than one resonance mode present over the magnetic field range investigated. 1. Low (0ËHË10 T)-field range
FIG. 2. ESR spectra for BiFeO3 at T⫽4.2 K as a function of magnetic field between 0 and 25 T for various submillimeter frequencies between 115 and 365 GHz. The symbols 共1兲, 共2兲, and 共3兲 represent different absorption peaks: they are illustrated to guide the eyes with their shift with frequency.
115⬍ ⬍360 GHz. This figure shows dramatic changes in the ESR spectra for the various frequencies. At lower frequencies ⬎115 GHz, a single absorption peak was found at lower magnetic fields, as illustrated by an arrow 共1兲. With increasing , this absorption peak was continuously shifted to higher fields ( ⬃H) and the degree of absorption was increased, as illustrated by arrows labeled as 共1兲. Additional peaks were found in higher fields, denoted by arrows labeled as 共2兲 and 共3兲. Of particular interest was the peak indicated by arrows labeled as 共3兲 in Fig. 2, which became apparent for ⬎200 GHz. This resonance absorption was quite pronounced, and in fact the attenuation of the submillimeter radiation in the crystal at this resonance was significant. With increasing , this peak continuously shifted to higher H ( ⬃H), the adsorption became increasingly pronounced, and the peak became increasingly broad. Clearly, under high magnetic field, a secondary resonance state is induced. The shape of this secondary resonance peak is noticeably dependent upon H and . Resonance frequency vs H
The experimental observations of the dependence of the resonance frequencies on H are summarized in Fig. 3.
A low-field spin-resonance mode was observed that had a linear relationship between and H, which had a slope of ⬃27 GHz/T 共that corresponds to Lande g factor of ⬃2.0) and a slope intercept of zero. These data are illustrated in Fig. 3 using closed circle symbols and dashed line. This is the spin-resonance mode that corresponds to the arrows labeled as 共1兲 in Fig. 2. The cycloidal modulation has previously been measured by temperature-dependent NMR studies,17,18 but ESR studies are without precedent. The NMR studies revealed that the spin profile is anharmonic at 4.2 K, becoming increasingly sinusoidal with increasing temperature.17 2. Intermediate (10ËHË18 T)-field range
The low-field spin mode was found to continue until higher fields, maintaining the same slope value of g⬃2. However, an ‘‘intermediate-field range’’ of 10⬍H⬍18 T can be designated, based upon the presence of an additional resonance peak whose resonance frequency decreased with increasing H, as shown in Fig. 3 by the gray square symbols. This is an anomalous result as both the g factor and magnetic permeability are positive. In addition, hysteretic effects became very pronounced between ESR spectra obtained on increasing vs decreasing H sweeps. This is further illustrated in Fig. 4, which shows a representative ESR signal taken at a measurement frequency of 236 GHz. In this figure, significant hysteretic effects were found in the intermediate field range of 10⬍H⬍18 T. Hysteresis effects are known in pinned incommensurate structures, see, for instance, in the field-induced incommensurate phase of CuGeO3 . 41,42 The data support a model of an incommensurately modulated cycloidal structure whose spin profile is changed
PHYSICAL REVIEW B 69, 064114 共2004兲
BENJAMIN RUETTE et al.
phase transition of BiFeO3 and changes in the ESR spectra will then be given. The Landau-Ginzburg energy19 of the spin structure of BiFeO3 is the sum F⫽F L ⫹F exch ⫹F an ⫹F m ,
where F L is the magnetoelectric coupling that is linear in gradient, in which the Lifshitz invariant is responsible for the creation of the spatially modulated spin structure, F exch is the inhomogeneous exchange energy, F an is the anisotropy energy, and F m is the magnetic energy. We have formulated a solution to the LG equation,43– 45 whose derivation can be found in the EPAPS system.46 The volume-averaged free energy of the spin cycloid state (F cycloid), under a magnetic field parallel to the 关 001兴 c direction of H⫽(H x ,0,H z ), is F cycloid⫽⫺ ⬜ FIG. 4. Representative ESR signal illustrating hysteretic effects ជ ⬍18 T. The closed present in the intermediate field range of 10⬍H line was taken on increasing field sweep, and the dashed line was taken on decreasing field sweep.
by application of H. The spiral structure becomes increasingly anharmonic with increasing H as an induced phase transition is approached. In addition, the spin cycloid may become depinned with increasing H, resulting in hysteretic effects. 3. High-field range of HÌ18 T
Figure 3 clearly demonstrates an induced phase transition near H⫽18 T. In the high-field range, a secondary spinresonance mode was observed. These data are shown as open circles in Fig. 3. The slope of this secondary spin mode was ⬃ 12 of that of the low-field one, having a value of 13 GHz/T. No hysteretic effects were observed in the ESR spectra, within this secondary mode. It is important to notice that the primary 共low-field兲 spin mode can be linearly extrapolated into the high-field regime, revealing the presence of a field-induced gap state. Due to strong microwave absorption at higher frequencies, it was found difficult to experimentally confirm the linear extrapolation. However, the ESR spectra at 365 GHz clearly show this primary resonance persisting, which was of noticeable absorption. The data indicate an induced gap for H⬎18 T. To understand the nature of the secondary resonance mode, it is thus necessary to develop a theoretical approach. We conjecture that the induced phase transformation is from the cycloidal to a homogeneously magnetized state. In the following section, we shall present this theoretical formulation, and show supporting evidence. IV. LANDAU-GINZBURG THEORY FOR FIELD-INDUCED TRANSITION, AND ESR SPECTRA
In this section, a Landau-Ginzburg 共LG兲 formalism for the free energy will be considered. A theory for the field-induced
H2 1 Ku 5 共 ␤• Pz兲2 ⫺ ⫹ K 2 ⫺ ⬜ 共 ␣ • P z 兲2⫹ 2 4A 2 8 4 H z2 4
where ⬜ is the magnetic susceptibility of the media in the direction perpendicular to the antiferromagnetic vector ជl , A is a stiffness coefficient, ␣ is the inhomogeneous relativistic exchange constant 共inhomogeneous magnetoelectric constant兲, P z is spontaneous polarization, K u is the uniaxial magnetic anisotropy constant, K 2 is the second-order anisotropy, and ␤ is the homogeneous magnetoelectric constant 共i.e., a magnetoelectriclike Dzyaloshinsky-Moria, or DM, interaction兲. A phase transition to the homogeneous antiferromagnetic spin state will occur at a critical field H c , when the energy of the homogeneous state is equal to that one of the cycloidal one. The energy of the homogeneous antiferromagnetic state (F homogenous), under an external field of H ⫽(H x ,0,H z ), is F homogenous⫽⫺
⬜ •H 2 共 ␤• Pz兲2 ⫹K u ⫹K 2 ⫺ ⬜ 2 2
⫺ ⬜ 共 ␤ • P z 兲 H x .
The dynamic properties of the cycloidal spin modulated and of the induced homogeneous antiferromagnetic spin states can be predicted by a Lagrangian method; again see EPAPS system for details.46 The ESR resonance frequency for fields of H⬎H c is
⫺b⫾ 冑b 2 ⫺4c 2
2K u ⫺H z2 ⫺ 共 ␤ • P z 兲 2 ⫺2 共 ␤ • P z 兲 H x ⫺H 2x , ⬜
2K u ⫺ 共 ␤ • P z 兲 2 ⫺H z2 ⫺ 共 ␤ • P z 兲 H x 共 ⫺H 2x ⫺ 共 ␤ • P z 兲 H x 兲 ⬜
⫺共 H xH z 兲2,
where ␥ ⫽1.73⫻10
冑cm/g is the gyromagnetic ratio.
PHYSICAL REVIEW B 69, 064114 共2004兲
MAGNETIC-FIELD-INDUCED PHASE TRANSITION IN . . . Predictions and supporting evidence
Equations 共4a兲–共4c兲 describe the magnetic-field dependence of the electron spin resonance frequency for a homogeneous spin state. It is not applicable to the cycloidal spin state, as the gradient terms were excluded; see EPAPS system.46 Equations 共4a兲–共4c兲 demonstrate that the resonant frequency of the homogeneous spin phase is dependent only upon two independent parameters: 共i兲
an anisotropic magnetic factor, given as Ku , and 共5a兲 ⬜ a polarization factor that is coupled to the magnetization m through the linear magnetoelectric coefficient ␤ of the homogenous spin ordered state, given as m 共5b兲 HDM⫽ ␤ • P z ⫽ , ⬜ where H DM is the Dzyaloshinsky-Moria field. In the homogeneous spin state, there will be a net magnetoelectric effect that is equal to ␤.
These two parameters can be obtained by fitting to the experimental data. Figure 3 shows the result of this fitting, illustrated as dashed lines. It yields values for the anisotropic magnetic factor of K u / ⬜ ⫽1.41⫻1010 erg/cm3 , and for the Dzyaloshinsky-Moria field of D⫽ ␤ • P z ⫽1.19⫻105 Oe 共or 11.9 T兲. The dashed curve, corresponding to the solution involving ⫺ 冑b 2 ⫺4c in Eq. 共4a兲, is in good agreement with the experimental data for fields above that of the induced phase transition (⬃18 T). Near, but below this field, there was an apparent noise in the data, due to hysteresis around the phase-transition point. Our solution cannot account for this hysteresis, as it does not apply for H⬍H c . The solution involving ⫹ 冑b 2 ⫺4c in Eq. 共4a兲 gives frequencies much greater than that of the upper limit of our experimental range, and thus has not been experimentally verified. The uniaxial anisotropy constant K u can also be calculated from the ESR data. Using the reported value47 for the perpendicular susceptibility of ⬜ ⫽4.7⫻10⫺5 , the uniaxial anisotropy constant can be approximated as K u ⫽6.6 ⫻105 erg/cm3 . Using values of H c ⫽1.8⫻105 Oe, A⬇8 ⫻10⫺7 erg/cm 共estimated from NMR data17兲, ␣ • P z ⫽2Aq, q⫽ 2 / , and ⫽620 Å, 15 the value of the second-order anisotropy constant can be approximated as K 2 ⬃104 erg/cm2 . The agreement of the theory and the high-field electron spin resonance mode demonstrates that the induced phase is the homogeneous antiferromagnetic spin state. The cycloidal spin structure is destroyed by increasing magnetic field, resulting in homogeneous spin order. The term homogeneous does not designate a single-crystal, single domain state which has homogenous order through out the specimen; such a condition only requires the Lifshitz invartiant term to be zero in the free-energy expansion. Rather, we use the term homogeneous to designate that the local pattern of spin arrangement is uniform within the domains. Accordingly, the spatial profile is uniform 共cycloidal structure de-
stroyed兲, and the magnetoelectric coefficients are not averaged to zero.
V. DISCUSSION AND SUMMARY
Bismuth ferrite at low fields has a cycloidal spin structure.15–19 The cycloidal structure is periodically modulated with ⬃600 Å. The spin profile is slightly anharmonic. To condense the homogeneously magnetized state requires the field-forced destruction of the long-wavelength cycloidal modulation. We have performed investigations of the electron spin resonance modes of BiFeO3 as a function of magnetic field. Studies were done up to very high magnetic fields 共25 T兲, sufficient to force the spin alignment, and to condense a homogeneous spin order. We summarize the observed changes in spin structure as follows. At low to moderate fields, a cycloidal spin structure exists. The profile and modulation wavelength of the cycloidal structure are changed with H. With increasing H, the incommensurate structure becomes depinned, resulting in hysteretic effects between increasing and decreasing H sweeps. Above some critical field H c , a transition to a homogeneously magnetized state is induced. This transition results in the destruction of the spin cycloid. Phenomenologically, the order parameter of the transition between the cycloidal and homogeneously magnetized states is dependent on the inhomogeneous and homogeneous magnetoelectric coefficients 共␣ and ␤, respectively兲. The ESR peaks in the homogeneous magnetized state were found to be quite broad, and in fact became increasingly broad with increasing H for H⬎H c , as can be seen in Fig. 2. Peak broadening of ESR and NMR spectra has previously been described using a multisoliton theory.23,25–29 Our results indicate that there may be numerous regions of homogeneously magnetized spin order. A. Comparison of our estimated value for ␤ with that recently reported for BiFeO3 thin layers
Recent investigations of 共001兲-oriented BiFeO3 epitaxial thin layers grown on strontium titanate have shown dramatically higher values of the spontaneous ( P s ) and remanent ( P r ) polarizations13 than for bulk single crystals. The saturation polarization of the thin layer can be seen to be ⬃0.52 C/m2 , which is much higher than the value of 0.035 C/m2 previously reported for 共001兲-oriented single crystals. In addition, the 共001兲-oriented BiFeO3 thin layers were reported to have dramatically higher magnetoelectric 共ME兲 coefficients,13 than the bulk crystals. The value of the ME coefficient of the thin layers in the remanently polarized and magnetized states is ⬃3.5 V/Oe cm. The significant changes in the magnetoelectric, ferroelectric, and ferromagnetic behavior of the thin layers might be understood in terms of an epitaxially induced homogeneously magnetized state. To support this possibility, we estimated the value of the magnetoelectric coefficient of the homogeneous spin state for the single crystal of
PHYSICAL REVIEW B 69, 064114 共2004兲
BENJAMIN RUETTE et al.
BiFeO3 from the measured value of H DM , comparing it to the reported value of the magnetoelectric coefficient of 共001兲-oriented BiFeO3 thin layers. Rearrangement of Eq. 共5b兲 gives the homogeneous ME coefficient 1/␤ in units of V/Oe m,
V Pz 1 ⫽ , ␤ 3 Oe m o KH DM
where o is the permittivity of free space and K is the relative dielectric constant which is equal to ⬃100.13 The value of 1/␤ 3 can be estimated from the measured value of H DM ⫽1.2⫻105 Oe in Fig. 3, and the inherent value of P z ⫽0.035 C/m2 of the single crystal.10 The value of 1/␤ 3 for the homogeneously spin ordered state is
冋 册 冋 册
In this investigation, we have reported experimental evidence of a high magnetic-field-induced phase transformation between a cycloidal and a homogeneous magnetized state in BiFeO3 . The field dependence of electron spin resonance modes have been theoretically predicted using LandauGinzburg theory that includes a relativistic antisymmetric exchange, and experimentally confirmed by high-field ESR measurements. The transformation between cycloidal and homogeneous spin orders is related to a Lifshitz invariant in the free-energy expansion that is magnetoelectric in nature. In both states, the magnetoelectric coefficient ␤ is the same, but the ME coefficient is only manifested in the homogeneous one.
V V 0.035 1 ⫽ ⫽3.3 . ⫺12 5 ␤ 3 8.85⫻10 ⫻100⫻1.2⫻10 Oe m Oe cm 共6b兲 Comparisons of the predicted value of 1/␤ 3 in Eq. 共6b兲 with the experimentally observed value in Ref. 13 of 3.5 V/Oe cm will demonstrate remarkable agreement. This indicates that a homogeneous spin state might be induced by either application of high magnetic field or by epitaxial constraint 共or alternatively by the influence of boundary conditions兲, suggesting the possibility to release the latent magnetoelectricity locked within the cycloid.
G. A. Smolenskii and I. Chupis, Sov. Phys. Usp. 25, 475 共1982兲. D. K. H. Salje, Phase Transitions in Ferroelastic and Co-elastic Crystals 共Cambridge University Press, Cambridge, 1990兲. 3 Yu. N. Venevtsev, G. Zhdanov, and S. Solov’ev, Sov. Phys. Crystallogr. 4, 538 共1960兲. 4 G. Smolenskii, V. Isupov, A. Agranovskaya, and N. Krainik, Sov. Phys. Solid State 2, 2651 共1961兲. 5 P. Fischer, M. Polomskya, I. Sosnowska, and M. Szymanksi, J. Phys. C 13, 1931 共1980兲. 6 G. Smolenskii, V. Yudin, E. Sher, and Yu. E. Stolypin, Sov. Phys. JETP 16, 622 共1963兲. 7 S. Kiselev, R. Ozerov, and G. Zhdanov, Sov. Phys. Dokl. 7, 742 共1963兲. 8 C. Michel, J-M. Moreau, G. D. Achenbach, R. Gerson, and W. J. James, Solid State Commun. 7, 701 共1969兲. 9 J. D. Bucci, B. K. Robertson, and W. J. James, J. Appl. Crystallogr. 5, 187 共1972兲. 10 J. R. Teague, R. Gerson, and W. J. James, Solid State Commun. 8, 1073 共1970兲. 11 Yu. E. Roginskaya, Yu. Ya. Tomashpol’skii, Yu. N. Venevtsev, V. M. Petrov, and G. S. Zhdanov, Sov. Phys. JETP 23, 47 共1966兲. 12 F. Kubel and H. Schmid, Acta Crystallogr., Sect. B: Struct. Sci. B46, 698 共1990兲. 13 J. Wang, H. Zheng, V. Nagarajan, B. Liu, S. B. Ogale, D. Viehland, V. Venugopalan, D. G. Schlom, M. Wuttig, R. Ramesh, J. B. Neaton, U. V. Waghmare, N. A. Hill, and K. M. Rabe, Science 299, 1719 共2003兲. 1 2
We gratefully acknowledge the support of the Office of Naval Research under Grant Nos. N000140210340, N000140210126, and MURI N000140110761, and to RFBR 01-02-1695. A portion of this work was performed at the National High Magnetic Field Laboratory, which is supported by NSF Cooperative Agreement No. DMR-0084173 and by the State of Florida.
J. Wang, B. Ruette, M. Wuttig, R. Ramesh, and D. Viehland 共unpublished兲. 15 I. Sosnowska, T. Peterlin-Neumaier, and E. Steichele, J. Phys. C 15, 4835 共1982兲. 16 I. Sosnowska, M. Loewenhaupt, W. I. F. David, and R. Ibberson, Physica B 180&181, 117 共1992兲. 17 A. Zalesskii, A. Zvezdin, A. Frolov, and A. Bush, JETP Lett. 71, 465 共2000兲. 18 A. V. Zalesskii, A. A. Frolov, T. A. Khimich, A. A. Bush, V. S. Pokatilov, and A. K. Zvezdin, Europhys. Lett. 50, 547 共2000兲. 19 I. Sosnowska and A. Zvezdin, J. Magn. Magn. Mater. 140-144, 167 共1995兲. 20 Yu. F. Popov, A. Zvezdin, G. Vorob’ev, A. Kadomtseva, V. Murashev, and D. Rakov, JETP Lett. 57, 69 共1993兲. 21 A. Kadomtseva, Yu. Popov, G. Vorob’ev, and A. Zvezdin, Physica B 211, 327 共1995兲. 22 Yu. F. Popov, A. Kadomteseva, S. Krotov, D. Belov, G. Vorob’ev, P. Makhov, and A. Zvezdin, Low Temp. Phys. 27, 478 共2001兲. 23 R. Blinc and A. P. Levanyuk, Incommensurate Phases in Dielectrics 共North-Holland, New York, 1986兲. 24 T. Lorenz, B. Buchner, P. H. M. van Loosdrecht, F. Shonfield, G. Chouteau, A. Revcolevschi, and G. Chalenne, Phys. Rev. Lett. 81, 148 共1998兲. 25 R. Blinc, U. Micac, T. Apih, J. Dolinsek, J. Seliger, J. Slak, S. Zumer, L. Guibe, and D. Ailion, Phys. Rev. Lett. 88, 015701 共2002兲. 26 B. Topic, U. Haeberlen, and R. Blinc, Phys. Rev. B 42, 7790 共1990兲. 14
PHYSICAL REVIEW B 69, 064114 共2004兲
MAGNETIC-FIELD-INDUCED PHASE TRANSITION IN . . . 27
R. Blinc, P. Prelovsek, and R. Kind, Phys. Rev. B 27, 5404 共1983兲. 28 T. Aphih, U. Mikac, J. Dolinsek, J. Seliger, and R. Blinc, Phys. Rev. B 61, 1003 共2000兲. 29 T. Aphih, U. Mikac, J. Seliger, J. Dolinsek, and R. Blinc, Phys. Rev. Lett. 80, 2225 共1998兲. 30 H. Schmid, Int. J. Magn. 4, 337 共1973兲. 31 H. Schmid, Ferroelectrics 252, 41 共2001兲. 32 V. Dubovik, S. Krotov, and V. Tugusheve, Sov. Phys. Crystallogr. 32, 314 共1987兲. 33 E. Ascher, Magnetoelectric Interaction Phenomena in Crystals, edited by A. Freeman and H. Schmid 共Gordon and Breach, New York, 1975兲, p. 69. 34 Yu. M. Sirotin and M. P. Shaskol’skaya, The Fundamentals of Crystallography 共Nauka, Moscow, 1975兲. 35 V. Ginsburg, A. Gorbatsevich, Yu. Kopaev, and B. Volkov, Solid State Commun. 50, 339 共1987兲. 36 J. Ohtani and K. Kohn, J. Phys. Soc. Jpn. 53, 3744 共1984兲. 37 R. Birss, Symmetry and Magnetism 共North-Holland, Amsterdam, 1964兲. 38 C. Tabares-Munoz, J. Rivera, A. Bezinges, A. Monnier, and H. Schmid, Jpn. J. Appl. Phys., Part 1 24, 1051 共1984兲.
V. Eremenko, A. V. Klochko, V. M. Naumenko, and V. V. Pishko, JETP Lett. 40, 986 共1984兲. 40 S. A. Zvyagin, J. Krzystek, P. H. M. van Loosdrecht, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 67, 212403 共2003兲. 41 W. Palme et al., Phys. Rev. Lett. 76, 4817 共1996兲. 42 S. A. Zvyagin 共unpublished兲. 43 L. D. Landau and E. M. Lifshitz, Statistical Physics. Course of Theoretical Physics 共Pergamon, Oxford, 1997兲, Vol. V. 44 M. M. Tehranchi, N. F. Kubrakov, and A. K. Zvezdin, Ferroelectrics 204, 181 共1997兲. 45 A. K. Zvezdin and A. Mukhim, JETP 102, 577 共1992兲. 46 See EPAPS Document No. E-PRBMDO-69-019406 for supplementary material on the Landau-Ginzburg formalism. A direct link to this document may be found in the online article’s HTML reference section. The document may also be reached via the EPAPS homepage 共http://www.aip.org/pubservs/epaps.html兲 or from ftp.aip.org in the directory /epaps/. See the EPAPS homepage for more information. 47 Z. V. Gabbasova, M. D. Kuz’min, A. K. Zvezdin, L. S. Dubenko, V. A. Murashov, D. N. Rakov, and I. B. Krynetsky, Phys. Lett. A 158, 491 共1991兲.